Presentation on theme: "MECHANICAL PROPERTIES OF MATERIALS"— Presentation transcript:
1 MECHANICAL PROPERTIES OF MATERIALS Manufacturing Processes, 1311Dr Simin NasseriSouthern Polytechnic State University
2 MECHANICAL PROPERTIES OF MATERIALS Stress‑Strain Relationships (Slide 4)Tensile Test (Slide 7)Compression Test (Slide 36)
3 Mechanical Properties in Design and Manufacturing Mechanical properties determine a material’s behavior when subjected to mechanical stressesProperties include elastic modulus, ductility, hardness, and various measures of strengthDilemma: mechanical properties desirable to the designer, such as high strength, usually make manufacturing more difficultThe manufacturing engineer should appreciate the design viewpointAnd the designer should be aware of the manufacturing viewpointManufacturing engineerDesigner
5 Stress‑Strain Relationships Three types of static stresses to which materials can be subjected:Tensile - tend to stretch the materialCompressive - tend to squeeze itShear - tend to cause adjacent portions of material to slide against each otherStress‑strain curve - basic relationship that describes mechanical properties for all three types
7 Tensile TestMost common test for studying stress‑strain relationship, especially metalsIn the test, a force pulls the material, elongating it and reducing its diameterFigure 3.1 Tensile test: (a) tensile force applied in (1) and (2) resulting elongation of material
8 Tensile Test SpecimenASTM (American Society for Testing and Materials) specifies preparation of test specimenFigure 3.1 Tensile test:(b) typical test specimen
10 Tensile Test Sequence Figure 3.2 Typical progress of a tensile test: If pieces are put back together as in (6), final length can be measured(1) beginning of test, no load(2) uniform elongation and reduction of cross‑sectional area(3) continued elongation, maximum load reached(4) necking begins, load begins to decrease(5)fracture
12 Different types of stress-strain graphs Engineering important in designStress-strain curvesTrue important in manufacturing
13 Engineering Stress Defined as force divided by original area: where e = engineering stress (MPa) or Pa or psi,F = applied force (N) or lb, andAo = original area of test specimen (mm2 or m2 or in2)(Remember: N/ m2 = Pa, N/ mm2 = MPa,lb/ in2 = psi, klb/ in2 = kips/ in2)
14 Engineering Strain Defined at any point in the test as where e = engineering strain (it has no unit);L = length at any point during elongation; andLo = original gage length
15 Typical Engineering Stress-Strain Plot Figure 3.3 Typical engineering stress‑strain plot in a tensile test of a metal.
16 Two Regions of Stress‑Strain Curve The two regions indicate two distinct forms of behavior:Elastic region – prior to yielding of the materialPlastic region – after yielding of the material
17 Elastic Region in Stress‑Strain Curve Relationship between stress and strain is linearMaterial returns to its original length when stress is removedHooke's Law: e = E ewhere E = modulus of elasticity, e = stress, e=strainE is a measure of the inherent stiffness of a materialIts value differs for different materials
18 Yield Point in Stress‑Strain Curve As stress increases, a point in the linear relationship is finally reached when the material begins to yieldYield point Y can be identified by the change in slope at the upper end of the linear regionY = a strength propertyOther names for yield point = yield strength, yield stress, and elastic limit
19 Plastic Region in Stress‑Strain Curve Yield point marks the beginning of plastic deformationThe stress-strain relationship is no longer guided by Hooke's Law (non-linear relationship)As load is increased beyond Y, elongation proceeds at a much faster rate than before, causing the slope of the curve to change dramatically
20 Tensile Strength in Stress‑Strain Curve Elongation is accompanied by a uniform reduction in cross‑sectional area, consistent with maintaining constant volumeFinally, the applied load F reaches a maximum value, and engineering stress at this point is called the tensile strength TS (or ultimate tensile strength)TS =
21 Ductility in Tensile Test Ability of a material to plastically strain without fractureDuctility measure = elongation ELwhere EL = elongation (expresses as a percent);Lf = specimen length at fracture; andLo = original specimen lengthLf is measured as the distance between gage marks after two pieces of specimen are put back together
22 Area reduction defined as expressed as a percent, where: Af = area of the cross section at the point of fracture, mm2 or in2A0 = original areaTherefore, ductility is measured by elongation (EL) or area reduction (AR).
23 Lets compare! Which material has the highest modulus of elasticity? Which material has the highest tensile strength?Which material has the highest elongational rate?
24 LOW - - - - - - - - - - - - - - - - - - - - - - - - > HIGH Lets compare!LOW > HIGHModulus of elasticity (measure of stiffness):Polyethylene (0.03x106 psi), Nylon, Lead (3x106 psi), Magnesium, AL & Glass, Copper, Cast Iron (20x106 psi), Iron & Steel (30x106 psi), Alumina (50x106 psi), Tungsten, Diamond (150x106 psi)stresshas lower EstrainFor a given force, the one with lower E, deforms more in comparison with the one with higher E (which is stiffer).
25 LOW - - - - - - - - - - - - - - - - - - - - - - - - > HIGH Lets compare!LOW > HIGHTensile Strength:AL (10,000psi), Copper, Cast Iron (40,000psi), Mg, Low C Steel, High C Steel(90,000psi), Stainless steel (95,000psi), Ti alloyElongation:Metals: Cast Iron (0.6%), Mg, high C steel (10%), Ti, low C steel (30%), Nickel, Stainless steel (55%).Ceramics: 0%Polymers: thermosetting polymer (1%), Thermoplastic polymer (100%)
26 In elastic region they are almost the same True StressStress value obtained by dividing the applied load by the instantaneous areaIn elastic region they are almost the samewhere = true stress;F = force; andA = actual (instantaneous) area resisting the load
27 True Strain or Hencky strain Provides a more realistic assessment of "instantaneous" elongation per unit length
28 True Stress-Strain Curve Figure 3.4 ‑ True stress‑strain curve for the previous engineering stress‑strain plot in Figure 3.3.
29 Strain Hardening in Stress-Strain Curve Note that true stress increases continuously in the plastic region until neckingIn the engineering stress‑strain curve, the significance of this was lost because stress was based on an incorrect area valueIt means that the metal is becoming stronger as strain increasesThis is the property called strain hardening
30 True stress versus Engineering Stress True strain can be related to the corresponding engineering strain by:True stress and engineering stress can be related by the expression:Flow curveTrue stress versus true strain in plastic region:K is the strength coefficient and is in MPa. n is the strain hardening exponent.
31 Flow Curve True stress-strain curve a straight line in a log-log plot: Figure 3.5 True stress‑strain curve plotted on log‑log scale.
32 Engineering Stress & strain Lets compare!Engineering Stress & strainTrue Stress & strainElastic regione = E eTS =TS =Plastic region
33 Lets compare!Toughness: area under strain-stress graph (combination of ductility and strength)
34 Categories of Stress-Strain Relationship Perfectly elasticElastic and perfectly plasticElastic and strain hardening
35 Perfectly ElasticBehavior is defined completely by modulus of elasticity EFractures rather than yielding to plastic flowBrittle materials: ceramics, many cast irons, and thermosetting polymersFigure 3.6 Categories of stress‑strain relationship:(a) perfectly elastic.
36 Elastic and Perfectly Plastic Stiffness defined by EOnce Y reached, deforms plastically at same stress levelFlow curve: K = Y, n = 0Metals behave like this when heated to sufficiently high temperatures (above recrystallization)One example is LeadFigure 3.6 Categories of stress‑strain relationship:(b) elastic and perfectly plastic.
37 Elastic and Strain Hardening Hooke's Law in elastic region, yields at YFlow curve: K > Y, n > 0Most ductile metals behave this way when cold workedFigure 3.6 Categories of stress‑strain relationship:(c) elastic and strain hardening.
39 Compression TestApplies a load that squeezes the ends of a cylindrical specimen between two platensFigure 3.7 Compression test:(a) compression force applied to test piece in (1) and (2) resulting change in height.
41 Engineering Stress in Compression As the specimen is compressed, its height is reduced and cross‑sectional area is increasede = -whereAo = original area of the specimen
42 Engineering Strain in Compression Engineering strain is definedSince height is reduced during compression, value of e is negative(the negative sign is usually ignored when expressing compression strain)
43 Stress-Strain Curve in Compression Shape of plastic region is different from tensile test because cross section increasesCalculated value of engineering stress is higherIn comparison to the true stressFigure 3.8 Typical engineering stress‑strain curve for a compression test.
44 Tensile Test vs. Compression Test Although differences exist between engineering stress‑strain curves in tension and compression, the true stress‑strain relationships are nearly identicalSince tensile test results are more common, flow curve values (K and n) from tensile test data can be applied to compression operationsWhen using tensile K and n data for compression, ignore necking, which is a phenomenon peculiar to straining induced by tensile stressesBarreling and edge fracture happen